Upload
halel111
View
14
Download
0
Embed Size (px)
DESCRIPTION
SDFSDF
Citation preview
WOOD LAMINATED COMPOSITE POLES
A Dissertation Submitted to the Graduate School of the
Louisiana State University and Agricultural and Mechanical College
In partial fulfillment of the Requirements for the degree of
Doctor of Philosophy
in
The School of Renewable Natural Resources
by Cheng Piao
B.S., Northeast Forestry University, 1987 M.S., Northeast Forestry University, 1990
M.S., Louisiana State University, 1998 May 2003
ACKNOWLEDGEMENTS
Numerous individuals provided invaluable help throughout this project, which can
not be successfully completed without their invaluable assistance. I am sincerely grateful
to Dr. Todd Shupe, my major professor, for his guidance, advice, and assistance. My
deep appreciation is also extended to my other committee members. Specifically, I would
like to express my sincere gratitude to Dr. Chung Y. Hse for his guidance and advice
throughout this study. I am grateful to Dr. Vijaya Gopu, for his support and invaluable
advice on numerous subjects. Dr. C. F. Niels DeHoop served as a committee member for
my Master Degree and this degree and I would like to thank him for his assistance and
support. I also appreciate Dr. Arnold Bouma for his critical review of this dissertation.
I wish to express my appreciation to Dr. R. C. Tang for his help and guidance on
the test methodology of this project. Further appreciation is given to the following
persons: Ms. Patricia Lefeaux and JoAnn V. Doucet for their various assistance, Xiaobo
Li, Yaojian Liu, Dale Huntsberry, and Gary Smith for their assistance during the test of
specimens, and Steve Johnson for providing testing equipment. I give my appreciation
with fond memory to Dr. Elvin Choong for his support, assistance, and advice on this
project.
I thank my wife, Xiru Yang, whose patience and support were a constant source
of encouragement.
I am indebted to the Louisiana Forest Products Laboratory for funding this study
and my assistantship at Louisiana State University.
ii
TABLE OF CONTENTS
ACKNOWLEDGEMENTS ii LIST OF TABLES .. v LIST OF FIGURES .... vii ABSTRACT .. x INTRODUCTION ...... 1 CHAPTER 1 LITERAT ...... 5 URE REVIEW 1.1 References ....... 9 CHAPTER 2 MANUFACT . 11 URE AND EVALUATION OF COMPOSITE POLES
2.1 Introduction . 11 2.2 Strip Size Determination ...... 13 2.3 Experimental Procedure ... 15
2.3.1 Experimental Variables an ... 15 d Design 2.3.2 Materials and Methods ... 17
2.3.2.1 Specimen Preparation ... 17 2.3.2.2 Manufacture of Composite Pol 19 es
... 2.3.2.3 Manufacture of Control Poles 20 2.4 Tests ..... 20
2.4.1 Flexural Test ... 20 2.4.2 Glue-line Shear ... Test 25
2.5 Results and Discussion ... 26 2.5.1 Bending Stress ... 26 2.5.2 Modulus of Elasticit ..... y 30 2.5.3 Glue ... 33 -line Shear
2.6 Conclusions ... 38 2.7 References ........ 39
CHAPTER 3 THEORETICAL MODELS OF LAMINATED WOOD COMPOSIT ...... 40 E POLES
3.1 Introduction ..... 40 3.2 High-Order Differential Equations ..... 42 3.3 Solutions Based on Ti moshenko Beam Theory 49 3.4 Experimental Study ... 53 3.5 Results and Discussions ... 54
iii
3.5.1 Results of Theoretical Study .... 54 3.5.2 Comparison w .. 6 ith Experimental Results 53.5.3 Discussions .... 60
3.6 Summary and Conclusions .... 62 3.7.1 A Brief Summ . 62 ary of Model Development 3.7.2 Conclu ..... 63 sions
3.7 References ....... 64 CHAPTER 4 FINITE EL ... 67 EMENT ANALYSIS
4.1 Introduction ..... 67 4.2 Basic Theories ... 68 4.3 Discretization of Dom .... 73 ain 4.4 Material Properties ... 74 4.5 ANSYS Procedures ... 75 4.6 Experime ... 78 ntal Study 4.7 Results ... 78
4.7.1 Results of Finite Element Solutions ... 78 4.7.2 Comparison with Experimental Result ...
s 80
4.7.3 Com . 83 parison with Theoretical Results 4.8 Discussions ..... 86
4.9 Conclusions ..... 87 4.10 References ....... 88
APPENDIX: DETAIL DERIVATION OF THE THEORETICAL ANALYSIS .. 92 VITA ....... 97
iv
LIST OF TABLES
Table 2.1. Experiment variables and their levels of wood composite poles. . 16 Table 2.2. Strip parameters of wood composite poles. . 16 Table 2.3. Failure styles of solid and composite poles in a cantilever bending test. 24 Table 2.4. Shear stress of wood laminated composite poles in the cantilever bending
test. .. 27 Table 2.5. Maximum bending stress of small-scale wood laminated composite poles. 29 Table 2.6. Flexural properties of the small-scale solid poles. ... 29 Table 2.7. Modulus of elasticity of small-scale wood laminated composite poles. 30 Table 2.8. Modulus of elasticity of full-sized laminated composite poles. .. 31 Table 2.9. Glue-line shear strength values before and after water soaking of small-scale
composite poles. .. 33 Table 2.10. Percentage of wood failure in the glue-line shear test of wood composite
poles. 34 Table 3.1. Coefficients of the deformation model of small-scale composite poles with
three levels of number of strips and four levels of strip thickness. 54 Table 3.2. Coefficients of the deformation model of full-size composite poles with
two levels of number of strips and three levels of strip thickness. . 54 Table 3.3. Comparison among the deflection values from experiment and theoretical
models of small-scale composite poles with three strip-number levels and four thickness levels subjected to a 222 N (50 lbs) load. .... 65
Table 3.4. Comparison among the deflection values from experiment and theoretical models of the full-size composite poles with two strip-number levels and three thickness levels subjected to a 133 N (30 lbs) load. ... 65
Table 3.5. Comparison between the maximum bending stress values obtained in
experiment and predicted by a high-order differential equation model of small-scale composite poles. .... 65
v
Table 4.1. Number of elements in each configuration of composite poles. .. 74 Table 4.2. Other mechanical properties of clear southern yellow pine wood. 75 Table 4.3. Comparison between the deflection values obtained in the experiment and
values predicted from finite element analysis of small-scale composite poles subjected to a 222 N (50 lbs) load. . 84
Table 4.4. Comparison between the deflection values obtained from the experiment
and the values predicted by the finite element method of the full-size composite poles subjected to the same load for both test methods. 84
Table 4.5. Comparison between the maximum bending stress values obtained in
experiment and predicted by a finite element method of small-scaled composite poles. .. 85
Table 4.6. Comparison of strain values obtained from the attached strain gages to
those predicted from finite element analyses of the full-sized composite poles.89
Table 4.7. Comparison between the deflection values obtained in the theoretical analysis
and values predicted from finite element a te nalyses of small-scaled composipoles subjected to a 222 N (50 lbs) load. ... 89
Table 4.8. Comparison between the deflection values obtained from the theoretical
analysis and the values predicted by the finite element method of the full-size composite poles subjected to the same load for both test methods. .90
Table 4.9. Comparison between the maximum bending stress values obtained in the
theoretical analysis and predicted by the finite element method of small-scale composite poles. ..90
Table 4.10. Comparison between the deflection values obtained in the experiment
and values predicted from finite element analyses of small-scale poles (1.0 cm (0.4 in) and 1.5 cm (0.6 in) thickness) subjected to a 89 N (20 lbs) load. ...91
vi
LIST OF FIGURES
Figure 2.1. A schematic diagram of a wood strip composite pole and one of its strips.. 14 Figure 2.2. A schematic diagram of a strip-cutting plan for a nine-strip composite
pole. 18 Figure 2.3. A schematic diagram of the flexural testing device. 21 Figure 2.4 A schematic diagram of the clamp and mold that were used in the
flexural test. . 21 Figure 2.5 A strain gage was attached on the top skin of a small-scale spruce solid
pole. 22 Figure 2.6 A full-size composite pole is testing by a REVEL machine. 24 Figure 2.7 A schematic diagram of a sample cutting plan of the glue-line shear test... 26 Figure 2.8. Effects of strip thickness and number of strips on the shear stress of
small-scale wood composite poles. ... 28 Figure 2.9 Effects of strip thickness and number on the modulus of elasticity of
small-scale wood laminated composite poles. 32 Figure 2.10 Effects of strip thickness and number of strips on the glue-line shear
strength of wood composite poles. 35 Figure 2.11 Effects of strip thickness and number of strips on wood failure in the
glue-line shear test of wood composite poles. . 35 Figure 2.12 Effects of number of strips and thickness on the shear strength of wood
composite pole samples after a 2-hour boiling test. 37 Figure 2.13 Effects of strip thickness and number on the wood failure of composite
poles in the shear test after a 2-hour boiling treatment. 37 Figure 3.1 A schematic diagram of a wood composite pole and its coordinate. ... 42 Figure 3.2 A loading system, and shear and moment distribution of a cantilever beam..43
vii
Figure 3.3 A schematic diagram of the cross section of a 12-strip pole shell. ... 46 Figure 3.4 Deflection of 12-sided small-scale composite poles predicted by a high-order
differential equation model. .. 57 Figure 3.5 Deflection of 12-sided full-size composite poles predicted by a high-order
differential equation model. .. 57 Figure 3.6 Comparison of deflection of 12-sided small-scale composite poles
predicted by a high-order differential equation and Timoshenko beam models. 58
Figure 3.7 Deflection of 12-size full-size composite poles predicted by high-order
differential equation and Timoshenko beam models. ... 58 Figure 3.8 Effects of strip thickness and number of strips on the shear deflection of
small-scale composite poles. . 59 Figure 3.9 Stress distribution of small-scale composite poles with 12-sided and
2.0 cm (0.8 in) thickness subjected to a 445 N (100 lbs) concentrated load and a uniform body force. 66
Figure 4.1 Discretization and application of loads in the finite element analysis
of wood composite poles using ANSYS. 74 Figure 4.2 An ANSYS numbering system in the finite element analysis of wood
composite poles. . 79 Figure 4.3 Deformation of a wood composite pole in the solution of finite element
analysis using ANSYS. .. 79 Figure 4.4 Stress distribution of a wood composite pole in the finite element analysis
using ANSYS. .. 80 Figure 4.5 Deflection of 12-sided small-scale composite poles predicted by a finite
element model. .. 81 Figure 4.6 Deflection of 12-strip full-size composite poles predicted by a finite
element model. .. 81 Figure 4.7 Maximum bending stress of small-scale 12-sided composite poles with 4
strip thickness levels. Predicted by a finite element model. . 82
viii
Figure 4.8 Strain of 12-strip small-scale composite poles predicted by a finite element model under a 133 N (30 lbs) concentrated load. ... 82
Figure 4.9 Variation of deflection among the experimental, theoretical, and finite
element values for the small-scale composite poles with 12 strips. ... 91
ix
ABSTRACT
Wood composite poles are new engineered products with polygonal shapes and
bonded with synthetic resins. The poles have multiple advantages over the solid wood
poles and are a promising solid pole substitute in power transmission,
telecommunication, and cable TV services. The use of composite poles may reduce the
cost both in materials and manipulation, and facilitate installation and treatment. It is
necessary to evaluate the factors that affect their properties and construct theoretical and
analytical models to analyze these properties.
Experiments were conducted to investigate strip thickness and number of strips
(NOS) effects on the flexural properties and shear stress of wood composite poles.
Small-scale (diameter = 7.6 cm (3 in), length = 1.16 m (48 in)) and full size poles
(diameter = 10.2 cm (4 in), length = 6 m (20 ft) were manufactured for this purpose.
Four strip thickness levels and three number-of-strip levels for the small-scale poles, and
three thickness levels and two number-of-strip levels for full-size poles were chosen as
experimental variables. The lumber was cut into strips, which were bonded with
synthetic resin in molds, and the resulting poles were evaluated in a cantilever test.
Results show that the effects of strip thickness were negative on glue-line shear and
positive on the shear at poles clamped ends. But thickness had little effects on
maximum bending stress of the small-scale poles and Youngs modulus of both full- and
small-scale poles. With the increase of NOS, Youngs modulus of poles was increased.
NOS had little effects on the maximum bending stress and glue-line shear of small-scale
poles.
x
A theoretical analysis was carried out to study the deflection and stress of
composite poles. Governing differential equations were derived from high-order
differential equations based on the principle of minimum potential energy theorem.
Transverse shear and body forces were included in the model. Investigations were also
carried out to find glue-line effects on the stress and deflection of composite poles. An
analytical solution is modeled with the finite element analysis using ANSYS. Both
theoretical and analytical solutions were verified by the experimental data.
xi
INTRODUCTION
The use of wood poles in communication systems dates back to 1844, when the
first commercial telegraph system was constructed from Washington, D.C., to Baltimore,
Maryland (Panshin et al. 1950). This marked the beginning of pole production in the
forest-products industry. After about 40 years, poles were first used in another
transmission system - the electrical power transmission lines. Wood poles are now
widely used in communication and power transmission systems around the world. In
1998, about 130 to 150 million wood poles were used to carry overhead cables for
electric, telephone and cables in the United States (Canadian Institute of Treated Wood
(CITW) 1998). Both communication and electrical companies consume about two
million wood poles in annual construction of new lines. One to two millions of poles are
used to replace poles in service due to decay and/or mechanical damage (Erickson 1994).
Wood is an ideal material for poles. With the development of new materials and
processing techniques, poles made from materials other than wood entered in the
transmission and distribution markets. Spun concrete, light duty steel, and fiberglass are
the three important sources of such materials. Since wood is subject to rot, decay and
degradation from insects and woodpeckers, all of these materials are more durable than
wood. Moreover, the weight of fiberglass poles is even lighter than wood poles.
Nonetheless, wood is still the material of choice for poles in the U.S. This is due to the
intrinsic attributes of wood. Compared to other poles materials such as steel and
concrete, wood is produced from a renewable natural resource, which is resilient and
extremely resistant to oxidation, corrosion, fatigue, crumbling, and spalling. If properly
1
preservative-treated, wood is protected against the biological agents that cause it to
weaken and collapse in nature, namely: fungi and termites. Wood poles are easily
climbed, more than adequately strong and easily machined. The decisive factor that
wood is preferred over other materials is its low cost. Engineering Data Management
Inc. (EDM) compared life-cycle costs of four types of poles (wood, light-duty steel,
fiberglass (FRT), and spun concrete), and the results indicated that wood poles are the
least expensive life-cycle choice in most distribution pole categories (AWPI, 1996).
Although post-construction costs, such as inspection, maintenance, repair, replacement,
and disposal, are higher, wood poles remain the cost-effective choice.
However, due to the ever-increasing population and demand for wood, logs that
are suitable for transmission and distribution poles are becoming increasingly scarce.
The availability of this pole-size timber has severely diminished (Marzouk et al. 1978;
Miller and Graham 1970). On one hand, the wood pole industry faces the challenges of
rising cost and losing market share. On the other hand, the power companies have tried
to find a satisfactory substitute for the solid wood pole.
Orthotropic and laminated wood composite poles may be one of the solutions to
the current pole resource problem. Wood composite poles consist of wood strips bonded
with synthetic resin. The poles have polygonal cross-sections and a tapered form. Since
the strip thickness is less than pole radius, composite poles are hollow inside. For a pole
with a specific diameter, number of strips (NOS) and strip thickness are variables; for
different applications, composite poles can be made into any diameter and length. Pole
strips are normally finger- or butt-jointed to make them to pole length. The glue used is
resorcinol-formaldehyde resin, which is weatherproof and can set at room temperatures.
2
There are multiple advantages of composite poles over solid wood poles. It
normally takes 50 to 60 years for a tree to grow to a pole size. For composite poles, the
strips can be materials of various ages and sources. Therefore, the material cost of
composite poles is much lower than solid poles. The weight of hollow composite poles
can be half or even less than that of solid wood poles. This not only reduces processing
and transportation costs but also facilitates installation and transportation. In
manufacturing composite poles, lumber from low-grade trees and recycled poles can be
utilized. The disposal cost of solid poles can be greatly reduced by recycling into
composite poles. Wood from plantation-grown trees, small diameter trees, short logs,
crooked logs, and some processing residuals can be utilized as composite pole materials.
For composite poles, preservative treatment is simple to be carried out. When solid poles
are treated, since preservatives cannot reach the core, checks often occur during the
service and shorten the service time. This situation is unlikely to happen to composite
poles because of the size of the lumber and the permeability of plantation-grown wood
(Choong and Fogg 1972; Tesoro and Choong 1976; Simpson et al. 1988).
It is believed that there is a potential market for this composite product.
Utilization of low-grade timber bonded with high performance adhesives and fabricated
using the optimal structural design will allow wood composite poles to have a great
potential market and commercial values.
The objectives of this study are as followings:
1. Evaluate the mechanical properties of wood laminated composite poles.
2. Determine the factors that affect the mechanical properties of composite
poles.
3
3. Develop theoretical and finite element models to predict the loading behavior
properties of composite poles.
4
CHAPTER 1
LITERATURE REVIEW
Trees suitable for pole production must have long, straight, full-rounded boles
with little taper. The materials that meet these requirements are from various species.
Southern pine (Pinus, sp) is the main material for pole production in the nation. About
72 to 75 percent of poles are from this species (Koch 1972, Micklewright 1989). Other
species for poles are western red and northern white cedars, Douglas fir, chestnut,
Atlantic white cedar, bald cypress, and redwood (Panshin et al. 1950).
In the last decades, many new approaches have been designed to solve the pole-
resource-shortage problem. Marzouk et al. (1978) used four design schemes to make
shorter solid wood poles longer by splicing or strapping two to four shorter poles using
steel connectors. They presented three types of splicing and frame poles that are
structurally suitable substitutes for wood distribution power poles. They also investigated
the possibility of making composite poles from wood and concrete in which the top
position was made of pine and bottom position was made of concrete.
The concept of composite poles appears in 1981, when Adams et al. (1981)
fabricated an innovative product using wood flakes, synthetic resin, and preservatives,
and termed it the COMPOLE. The COMPOLE series are 40-foot long hollow poles with
square, hexagonal, or octagonal cross sections. This was the first time that the concept of
composite is applied in the field of wood poles. The poles they made are tapered from
butt to tip according to the range found in solid wood poles. A computer program was
used to design the poles and the optimal design they found was the poles that had a 7.5
5
cm (3 inches) wall thickness at a 33.8 cm (13.3 inches) ground-line diameter with the
octagonal cross section. Shell thickness was reduced to 2.5 cm (1 in) at the top.
Hollow poles have advantages over solid poles. Since the poles are hollow, the
poles are lighter in weight, which will save the cost in materials, shipping and
installation, compared with that of solid poles. From a mechanical analysis standpoint,
when a pole is subjected to a bending test, the bending stress is highest on the surface
layer and zero in the center part of the pole due to the effect of moment of inertia. Ninety
percent of a poles bending strength is attributable to 22 percent of its diameter on both
sides of the cross-section (Erickson 1995). Thus, taking some material from the center
part will not significantly affect the service strength of poles. A conventional inspection
method for poles in service also involves drilling to determine the shell thickness. A
distribution pole is designated a reject if the pole shell thickness is 5 cm (2 in) or less
(Wilson 1992). Examples like this can be found in the competitor to solid wood poles.
Most of poles made of steel, concrete, and fiberglass are hollow inside.
Mechanical properties and weathering properties are obviously the two important
factors that decided the application potential of COMPOLE. Krueger et al. (1982)
reported that the average bending strength and modulus of elasticity (MOE) of aligned
composite wood materials bound with isocyanate resin are 110.8 (16.1 x 103 psi) and
16,250 x 103 Pa (2.36 x 106 psi), which are higher than those of southern yellow pine.
The weight of COMPOLEs, however, is 50 percent of the weight of solid wood poles of
the same class and length (Adams et al. 1981).
Although weathering and biological attacks affect both COMPOLEs and solid
wood poles, COMPOLEs are more vulnerable to these attacks. Since preservatives are
6
added to flakes before hot pressing, preservatives had detrimental effects on the initial
strength properties of COMPOLEs. Test results showed that COMPOLEs lost some
strength after weathering tests (Krueger et al. 1982). The COMPOLEs that contain
inorganic salt-type preservatives had very high strength loss. They attributed the strength
loss to the high temperatures used in the accelerated weathering test and predicted that
the same results may not be seen in actual in-service weathering conditions. Wood
composites are normally pressed at high temperature and humid environments. The
built-in stress in the materials after pressed may release whenever it is possible. When
COMPOLEs are in an in-service application environment, they will be subjected to
constantly changes of moisture as well as temperature. The durability of COMPOLEs is
a real concern.
Erickson (1994, 1995) proposed and patented a new design of composite poles.
The hollow veneered pole (HVP) consists of a truncated strip cone with three or more
overwraps of veneer layers. NOS in the cone could be 8 or whatever is most appropriate
for the manufacture of a given sized pole. Each strip can be made from either random or
standardized lengths of lumber, and can be finger-jointed to pole length. The overwraps
are made of high strength softwood species veneer. Veneer grain direction is parallel to
the pole axis. The function of veneer layers is to improve the bending strength and
protect the glued surfaces of adjacent strips from weather.
There are no data reported about the mechanical properties of HVP. Since the
strips in HVP are made from solid wood, it can be expected that HVP will have better
mechanical properties and weathering ability than those of COMPOLE. Also the weight
of HVP should be less than that of the same size of COMPOLE because the density of
7
structural composite materials is always higher than the density of wood material. All
these make HVP an improvement on COMPOLE.
The wrapped veneer is the vulnerable part of the HVP. In the three-dimensional
configuration of wood, the strength of the tangential direction is substantially lower than
that of the longitudinal direction. When HVP swells due to the moisture changes in strips
and veneer, the veneer-wrap is easily checked and peeled off and loses its utility.
Furthermore, the over-wrap involves a complicated process of joining and gluing,
especially when the pole is tapered. It is reported that the cost of over-wraps accounts for
more than 20 percent of the total cost (Erickson 1994).
A merit of the substitutes to solid wood poles is sufficiently-strong strength and
stability for tens of years in adverse environments. Both COMPOLE and HVP do not
have these properties and may not be the most promising pole material. New designs are
needed to solve the pole material shortage and work as the substitute for solid poles. One
of the new designs is the wood laminated composite pole. In addition to the advantages
that both COMPOLE and HVP have, wood laminated composite poles are more cost-
effective, easier to make and be treated, more flexibility in sizes and shapes, especially,
more durable than COMPOLE and HVP. Furthermore, in the theory of poles and beams,
very few are found dealing with the hollow polygonal cross sections. The new design of
composite poles has glue-lines and longitudinal connections. Few theories are available
that take into account the effects of glue-lines and connections. Thus, a systematic study
is obviously needed to assess the physical and mechanical properties of wood laminated
composite poles. It is also imperative to develop theoretical and analytical models to
facilitate the manufacture, installation, and maintenance of the composite poles.
8
1.1 References
American Society for Testing and Materials. 1996. Standard methods of static test of wood poles, D 1036-58(64). American Institute of Timber Construction. Timber Construction Manual. 1974. John Wiley & Sons, New York. 928p. Choong, E.T. and P.J. Fogg. 1989. Differences in moisture content and shrinkage between innerwood and outerwood of two short-leaf pine trees. Forest Prod. J. 39(3):13-18. Canadian Institute of Treated Wood (CITW). 1998. Pole talk. Web address: www.citw.org/poletalk/. Dougherty, J.J. 1985. Electrical systems division R&D report. Wood poles structure design. EPRI Journal Dougherty, J.J. 1985. Electrical systems division R&D report. EPRI Journal (3):47-51. Koch, P. 1972. Utilization of the southern pines, Vol. 1, USDA For. Ser. Exp. Sta., Agric. Handbook 420, Washington DC. 1663p. Micklewright, J.T. 1991. Wood preservation statistics. Proceedings of the American Wood-Preservers Association 87:258-272. Marzouk, H. M., M. U. Hosain, and V. V. Neis. 1978. Built-up utility poles using prairie timber. Forest Prod. J. 28(11):49-54. Miller, D. J. and R. D. Graham. 1970. Durability of Douglas-fir hop poles treated with preservatives by diffusion. Forest Prod. J. 20(6):43-44. Roliadi, H., C.Y. Hse, and E.T., Choong. 1996. Recycling of utility poles for useful engineered wood products. V.K.A. Gopu (Editor), Proc. 4th International Wood Engineering Conference, Vol. 1, pp. 454-461, Oct. 28-31, 1996, New Orleans, LA. Roliadi, H. 1997. Recycling of utility poles for useful engineered wood products. Ph.D. Dissertation. Louisiana State University. Baton Rouge, LA. 201p. Simpson, W.T., J.D. Danielson, and R.S. Boone. 1988. Press-drying plantation-grown loblolly pine 2 by 4s to reduce warp. Forest Prod. J. 38(11/12):41-48. Tesoro, F.O. and E.T. Choong. 1976. Relationship of longitudinal permeability to treatability of wood. Holzforshung 30(3):91-96. Wood Preserving Industry Production Statistical Report. 1996. American Wood Preservers Institute. 2750 Prosperity Avenue, Suite 550, Fairfax, VA22031.
9
Panshin, A.J., E.S. Harrar, W.J. Baker, P.B. Proctor. 1950. Forest products: their sources, production, and utilization. McGraw-Hill Book Company, Inc.
10
CHAPTER 2
MANUFACTURE AND EVALUATION OF COMPOSITE POLES 2.1 Introduction
Since the first use in the nineteenth century, wood is still the raw material of
choice in todays distribution and communication pole market. However, with the
diminishing availability of pole-sized trees, pole industries face a shortage of material
and an increase in their cost. At the same time, the electrical and communication
companies are trying to find substitutes for solid poles. Laminated wood composite poles
are one important alternative for this purpose. These poles possess all the good properties
the solid wood poles have, such as climbability and machinablity. The weight of
composite poles is lighter than solid wood poles because the composite poles are hollow
inside. The cost of composite poles is less than solid wood poles. From a mechanics stand
point, if pole shell thickness is appropriate, hollow poles are still sufficiently strong to
meet strength requirements. Ninety percent of a poles bending strength comes from 22
percent of its diameter on both sides of the cross-section (Erickson 1995). Erickson
proved that for a 12.2 m (40 ft) Class 4 hollow veneered pole (HVP), saving of wood
could be 1/3 to 1/2 compared to solid poles. These properties make composite wood pole
a potential product in the pole market.
There are two designs in the current research of composite poles. The first design
uses wood flakes, synthetic resin, and preservatives to make poles (Adams et al. 1981).
There are some similarities between the manufacture of composite poles of this kind and
that of oriented strand board (OSB), in which the wood flakes with synthetic resin are
11
pressed under high temperature and pressure. Composite materials like this may store
stress in the poles due to elevated temperature, humidity, and pressure applied to poles
during manufacturing. The internal stress may be released whenever it is possible. The
durability of the poles is a concern when they are introduced to the constantly changing
outside environment. The second design consists of a wood strip cone over-wrapped by
single- or multiple-veneer layers (Erickson 1994, 1995). The cone is composed of 8 or
any appropriate number of strips (NOS), which are bound by synthetic resin side by side.
The poles are hollow; thus, strip thickness may be a variable. The functions of veneer
over-wraps were to protect the glue lines between strips and improve pole strength
properties (Erickson 1995). Because the veneer is easily checked and peeled off from the
poles, the over-wraps may not work as well as expected. The over-wraps account for
about 20 percent of the total cost and involve a complicated process, especially when
poles are tapered.
Wood laminated composite poles may be a better solution to the current problems
that are related to the shortage of large diameter and long length wooden poles and
beams. Laminated composite poles are thick-walled, polygonal shapes, and bamboo-like
beams, as contrasted to solid poles and laminated veneer lumber (LVL). The objective of
this part of study was to evaluate the factors that affect the physical and mechanical
properties of composite poles. As a pre-study of full-size composite poles, small-scale
poles were first made and tested. Full-size composite poles were made and tested based
on the information obtained in small-scale poles. Effects of NOS and strip thickness on
mechanical and water soaking properties were evaluated for both pole sizes.
12
2.2 Strip Size Determination
Strip size can be determined by mathematical calculation based on the parameters
given. The known parameters are NOS in a pole n, strip thickness T, radius (or
diameter) of the circle surrounding the bottom of a pole R, tapering angle , and pole
height H. Then the central angle can be calculated as
= 360o
n (2.1)
Other size measures can be determined by the relationship between sides and angles in a
triangle. Figure 2.1 shows a schematic diagram about a composite pole and one of its
strips. The formulas of other size are as followings:
Width of the larger size at pole bottom AB
AB R= 22
sin
(2.2)
Width of the smaller size at pole bottom CD
CD R T= 22
(sin tan )2
(2.3)
Width of the larger size at pole top AB
A B R H' ' ( tan ) sin= 22
(2.4)
Width of the smaller size at pole top CD
C DHR
RT
' ' ( tan )(cos
) sin= 2 12
2
(2.5)
Formulas 2.1 to 2.5 can be used to calculate the dimension of strips for a specific design
of composite poles.
13
D C B A
t
R
H
A B
C D
Figure 2.1. A schematic diagram of a wood strip composite pole and one of its strips.
14
If taper angle equals 0, i.e., there are no tapers in the pole, Equations 2.4
and 2.5 are the same as Equations 2.2 and 2.3, respectively.
2.3 Experimental Procedure
2.3.1 Experimental Variables and Design
Poles made in this study had no taper. Table 2.1 shows the experimental variables
and their levels. The small-scale poles (SSP) were used to simulate the properties of full-
size poles (FSP) and two variables were selected for this purpose. Since strip thickness
determines both strength properties and the cost, four and three levels were selected in
the design of SSP and FSP, respectively. The thickness of the SSP accounts for 26, 39,
52, and 66 percent of the pole radius for strip thickness of 1.0 cm (0.4 in), 1.5 cm (0.6 in),
2.0 cm (0.8 in), and 2.5 cm (1.0 in), respectively. For FSP thickness accounts for 38, 56,
and 75 percent of the pole radius for 1.9 cm (0.75 in), 2.9 cm (1.125 in), and 3.8 cm (1.5
in) strip thickness, respectively. Strip thickness covers one quarter to three quarters of
pole radius in this study. Number of strips (NOS) was chosen as multiplications of 3 to
facilitate calculations. SSP had three levels of NOS (6, 9, 12) and FSP had two (9, 12).
Solid SSPs were used to compare the composite poles to solid wood and to compare the
properties of different species. Two species were chosen, i.e., southern yellow pine and
spruce. The cross section of the solid poles was 6-, 9-, and 12-side polygons for both
southern yellow pine and spruce.
Table 2.2 presents the parameters for each NOS level of the strips with thickness
2.5 cm for SSP and 2.9 cm for FSP. The width of the larger side of other thickness levels
is the same.
15
Table 2.1. Experiment variables and their levels of wood composite poles.
Pole Types Species Diameter
(cm)
Length
(cm)
Thickness
Levels (cm)
Number of
Strips
Small-scale
composite
Southern yellow
pine 7.6 122
1.0, 1.5, 2.0,
2.5 6, 9, 12
Small-scale
solid
Spruce, southern
yellow pine 7.6 122 ------ 6, 9, 12
Full-size
composite
Southern yellow
pine 10.2 610 1.9, 2.9, 3.8 9, 12
Table 2.2. Strip parameters of wood composite poles.
Pole
Types
Number of
strips
Central
angle
(o)
Strip
thickness
(cm)
Width of larger
side
(cm)
Width of smaller
side
(cm)
6 60 2.5 3.81 1.27
9 40 2.5 2.61 0.87 Small-
scale poles 12 30 2.5 1.97 0.66
9 40 1.5 3.47 0.87 Full-size
poles 12 30 1.5 2.63 0.66
The experimental designs were factorial experiment designs for each experiment.
The number of experiments was 12 for the small-scale poles and 6 for full-size poles. For
RSP, thirty-six poles were made with 3 replications for each combination of NOS and
strip thickness levels; For FSP, 12 poles were made with 2 replications for the NOS and
strip thickness combinations. Three spruce and southern yellow pine poles were made
for each of the 6-, 9-, 12-sided configurations. Nine spruce and nine southern yellow
pine poles were used to test the properties of solid poles.
16
2.3.2 Materials and Methods
2.3.2.1 Specimen Preparation
Southern yellow pine (Pinus, sp) (SYP) lumber with sizes 5.08 cm by 15.36 cm
by 6.1 m (2 in x 6 in x 20 ft.) and 5.08 cm by 20.32 cm by 6.1 m (2 in x 8 in x 20 ft.) was
commercially obtained from a local store in Baton Rouge, Louisiana. Lumber pieces
chosen were those that had no large (diameter > 1 cm) live knots and no dead knots. The
lumber was randomly divided into two groups. One group was the materials for the RSP,
and one for the FSP. The lumber for the SSP was cut into 125 cm (4.1 feet) pieces and
reduced to target thickness with a planer. The lumber for the FSP was directly reduced to
target thickness with the planer. The resulting lumber was cut into strips of specific
target sizes using a table saw for both the SSP and FSP lumber pieces. The saw blade
was turned to appropriate angles shown in Table 2.2 to form the target angles in strips.
The cutting plan is shown in Figure 2.2. Strips may also be manufactured by first cutting
lumber into a rectangle then shaping to appropriate angles. A comparison of this plan
with the one shown in Figure 2.2 indicates that the latter may save some wood and
require less labor.
Each strip was inspected for quality after the strip was cut from lumber. Strips
with knots were removed and all strips were knot free. Strips were measured for weight,
width of the larger side, and stress-wave properties. The stress-wave data were used in
non-destructively assessing of the mechanical properties of poles. After measurement,
the strips were stacked in a constantly air-conditioned room for two weeks before gluing
into poles.
17
Figure 2.2. A schematic diagram of a strip-cutting plan for a nine-strip composite
pole.
18
2.3.2.2 Manufacture of Composite Poles
The glue used in this study was resorcinol-phenol formaldehyde (RPF) resin and
was commercially obtained from Borden Chemical, Inc. The viscosity and specific
gravity of RPF were 800 cps and 1.177, respectively.
Strips that were assigned to a pole were randomly selected from one group of
stacked strips for both SSP and FSP. Fifteen percent of setting agents was added to glue
and the mixture was blended in a mixer. The ready glue was uniformly hand-spread onto
the two side-surfaces at 310 g/m2 (63.3lbs/1000 ft2). Because both contacting surfaces
had glue, some of the excess glue was squeezed out from glue lines after pressure was
applied.
The consolidation of glued strips was performed in steel molds. The RSPs were
pressed in a 137 cm (4.5 ft.) length steel mold, and FSP in a 640 cm (20 ft.) length steel
mold. Glued strips were formed into a pole shape, tightened temporarily with tapes and
then put into the lower half of a steel mold with 91.44 cm (3 inches) inside diameter.
Rubber sheets were put in between poles and upper and lower halves of the steel mold.
An impact wrench with 48.4 kg m (350 lbs ft.) of torque was used to tighten the screws
on both sides of the steel mold. There were two functions of the rubber sheets. One was
to prevent the poles from sticking onto the steel. The other one was to provide a buffer
due to the pressure from steel to wood strips, and thus to prevent the mold from crushing
wood strips.
Poles were pressed in molds for 36 hours in an air-conditioning room. Poles were
then weighed and sanded. The poles were kept in an air-conditioned room for 4 weeks
before testing.
19
2.3.2.3 Manufacture of Control Poles
To compare the properties of composite poles and to test the dynamic properties
of solid wood poles, 6-, 9-, and 12-sided (polygonal) poles were made. Two materials
were used. One was the same material as those of composite poles, i.e., the southern
yellow pine; the other one was white spruce. Four pieces of 5.08 x 25.4 x 243.8 cm (2 in
x 10 in x 8 ft.) SYP and spruce lumber were commercially obtained from the same source
as the materials of the composite poles. The lumber was cut into 24 pieces of 5.08 x 7.6
x 121.9 cm (2 in x 3 in x 4 ft.) lumber. Two pieces of the lumber cut were bonded into
square wood with dimension of 7.62 x 7.62 x 121.9 cm (3 in x 3 in x 4 ft.) using
resorcinol-phenol-formaldehyde resin and 9 pieces of such square wood were obtained.
Three of the 9 pieces of square wood were cut into 6-sided polygonal posts, three into 9-
sided, and three into 12-sided posts for each species. The posts were kept in an air-
conditioned room for 4 weeks before testing. To test the dynamic properties and
facilitate the analysis of finite element of the solid poles, two strain gages were bonded
onto the top and bottom surfaces 5 cm (2 in) away from the clamp end. The strain gages
were connected to the Vishays Model 6010 Strain Gage Input Card and the Model 6100
Scanner, which is connected to a computer.
2.4 Tests
2.4.1 Flexural Test
The flexural tests were conducted on SSP and FSP and performed on a REVEL
machine. Before the test, the control system of the REVEL was replaced by a new digital
system, which is controlled by a computer. Figure 2.3 shows the set-up of the test.
20
In Figure 2.3, one end of the tested composite pole B is fixed in the clamp of the
supporting frame A. The pole was embedded 15 cm (6 in) in the clamp. The steel clamp
was lined with the maple, which gripped the pole. Figure 2.4 shows the cross-section of
the clamp, hard maple liner, and test specimen. The other end of the testing pole was tied
to the crosshead E of the REVEL through a steel cable C and a pully D. When testing,
the crosshead moved up along the spiral post F, imposing a concentrated load at the free
end of the pole. The test was controled by computer H and the testing data are collected
and stored in the computer.
G
H
E
F
C
D
B
A
Figure 2.3. A schematic diagram of the flexural testing device.
Steel clamp
Maple
Test specimen
Figure 2.4. A schematic diagram of the clamp and the hard maple line used to grip the test specimen.
21
Strain gages on the pole B in Figure 2.3 were used to record strain in the bending
test through software called StrainSmart. Figure 2.5 shows a strain gage attached to a
solid spruce pole during a bending test. The software scanned the strain gages 1,000
times per second.
Figure 2.5. A strain gage was attached on the top skin of a small-scale spruce solid pole.
To enhance the crushing strength of FSP at the fixed end, the hollow part of the
clamped end of each FSP was filled with thick plywood disks and glued particles. Two
thick polygonal plywood disks with 1.25 cm (0.5 in) thickness were cut for each FSP.
The disks were cut to fit the hollow part of each pole. Before the test, one disk was
pushed into the poles to 91 cm (3 ft) and stopped by a 3-cm (1.2 in) nail that was driven
in from the outside of the pole. The glued particles were then filled into the holes and
rammed with a steel rod. After the hole was totally filled, the second disk with glue on
22
the particle side was pushed in to seal the hole. The glue used was resorcinol-phenol-
formaldehyde resin. Resin content was 10 percent. After the operation, the poles were
kept at room temperature for 36 hours before testing.
Static bending tests were carried out for both solid and composite poles. The
experiment set-up is shown in Figure 2.3. Loading speed was 51 mm per minute (0.2
in/min). The length of the clamped end was 15.2 cm (6 in) for all the SSP and the length
of the FSP at the clamped end was 91.4 cm (3 ft). Peak load and deflection values were
recorded. The SSPs were tested twice. In the first test, all samples failed at the clamped
end, where the pole was split in the central plane. After the first test, the clamped ends of
the tested samples were removed. In the second test, the clamped length was increased to
30.5 cm (1 ft) and each sample was loaded to failure to obtain the maximum bending
stress. In the test of FSPs, strain gages were mounted on top and bottom skins near the
ground line and were used to measure strain during the loading process. FSPs were not
loaded to failure due to the subsequent experiment on the poles and were tested to obtain
only the modulus of elasticity (MOE). All FSPs were loaded to about 350 N (80 lbs) and
the test was halted. Load values and corresponding deflection and strain were recorded.
MOE was calculated from the load-deflection graph. Figure 2.6 shows a full-size
composite pole in the bending test. Table 2.3 gives the information of the bending test
for both small- and full-size poles.
After the second test on SSP, a sample was cut from the clamped end of each
pole. The samples were measured for weight and then put in an oven at 100oC for 24
hours. The moisture content at test was calculated based on the weight of the samples
before and after oven-drying.
23
Table 2.3. Failure styles of solid and composite poles in a cantilever bending test.
TYPES OF POLES NUMBER OF POLES FIRST TEST SECOND
TEST 1.0 cm 9 Shear1 Shear
1.5 cm 9 Shear Shear
2.0 cm 9 Shear Normal2 Composites
2.5 cm 9 Shear Normal
SYP 9 Normal -----
Small-scale
poles
Solid Spruce 9 Normal -----
1.9 cm 4 Non-destructive3 -----
2.9 cm 4 Non-destructive ----- Full-size poles Composites
3.8 cm 4 Non-destructive ----- 1 Shear failure at the clamped end. 2 Normal failure at the ground-line. 3 Loaded to about 350 N (180 lbs) and halted.
Figure 2.6. A full-size composite pole is loaded by a REVEL machine.
24
2.4.2. Glue-line Shear Test
After the bending test of each small-scale composite pole, the part measured 20
cm (8 in) from the clamped end of the pole was cut and kept for records. Four more
samples measuring 5 cm (2 in) each were cut from the same end and used for the glue-
line shear test. As shown in Figure 2.7, each sample was first cut into two halves. One
glue line was randomly selected from each of the halves. The laminations on both sides
of the glue line were reduced to 4.4 cm (1 in). Two of the samples were used to
determine the glue-line shear in the dry condition. The samples were kept in an air-
conditioned room for two weeks and tested to failure. The maximum load and wood
failure of each sample were recorded.
The other two samples for each pole were used to test in wet conditions. The
samples were put in a container measuring 36 x 72 x 23 cm (14 x 28 x 9 in). Water in the
container was heated to 50oC and the samples were put 2.5 cm (1 in) below the water
surface using a net. The water was heated to boiling point in two hours and samples were
kept in the boiling water for another two hours. At the end of the boiling test, the
samples were taken out and immediately put in plastic bags. After the samples cooled to
the ambient temperature in the bags, they were shear-tested to failure. The load to failure
and percentage of wood failure on the glue-line were recorded. The load values in the
wet condition and glue-line dimensions in the dry condition were used to calculate the
shear strength for each sample.
A standard apparatus was used to hold the samples and an Instron machine was
used to add the load. Before the test, each glue line in each sample was labeled, and
measured for length and width. Then the glue lines in the sample were tested to failure.
25
The testing procedure is similar to the standard ASTM D 1037 Glue-Line Shear Test
procedure except that the width of the samples was narrower because of the limited shell
thickness of the poles. The shear stress at failure was calculated based on the maximum
load and the glue line area, and the percentage of wood failure for each specimen was
recorded after the test.
Figure 2.7. A schematic diagram of a sample cutting plan for the glue-line shear test.
2.5. Results and Discussion
2.5.1 Bending Stress
In the first bending test, SSP samples were shear-broken at the clamped end. It
indicates that shear-failure may be an important failure mode for the hollow poles.
Therefore, some other materials may be needed to fill the void part and withstand the
shear effects.
The shear stress was calculated and Figure 2.8 and Table 2.4 show the results.
The shear values for the small-scale poles were normally higher than the wood itself.
This was due to the fact that the clamped end was pressed by the maple wood mold. As
shown in Figure 2.8, except for the 12-sided poles in the 2.0 and 2.5 cm groups, the
thickness of the poles had little effects on the shear stress of the poles.
26
Table 2.4. Shear stress of wood laminated composite poles in the cantilever bending test.
Shear Stress (MPa) Strip
Thickness (cm) 6 9 12
1.00 9.04 (0.17)* 9.69 (0.34) 9.79 (1.52) 1.50 8.11 (0.72) 11.81 (0.16) 10.34 (1.10) 2.00 8.22 (0.81) 10.42 (0.19) 13.47 (1.06) 2.50 8.32 (0.12) 11.45 (0.70) 12.44 (1.90)
* Values in parentheses are standard deviation.
Statistic analysis was conducted to analyze the effects of strip thickness and
number on the shear stress of composite poles. NOS had significant effects on the shear
stress at the clamped end (p = 0.001), but strip thickness showed no effects on the shear
stress (p = 0.15). The average shear stress values of 12 samples of each number-of-strip
level were 8.4, 10.8, and 11.5 MPa for 6-, 9-, and 12-sided poles, respectively. Least
significant difference (LSD) procedure was used to compare the effects among different
strip thickness and number-of-strip levels. This procedure is more conservative than
other procedures such as Tukey and Scheffe, i.e., LSD may differentiate small differences
caused by different levels in a variable. The shear stress was significantly lower than
those of other two number-of-strip levels. The average shear stress values were 9.5, 10.1,
10.7, and 10.7 MPa for poles with 1.0, 1.5, 2.0, and 2.5 cm of strip thickness,
respectively.
To test the bending stress of the small-scale poles, the clamped end of the pole
tested was removed after the first test and the poles were tested again. In the second test,
the clamped end was increased to 30.5 cm (12 in). Table 2.5 lists the results. In the test,
all poles in the 1.0 and 1.5 cm of thickness levels were failure by shear at the clamped
end, and poles in the other two thicker levels were failure at the ground line. There was
27
0
2
4
6
8
10
12
14
16
1.0 1.5 2.0 2.5
Strip Thickness (cm)
Shea
r Str
ess
(MPa
)
6-side
9-side
12-side
Figure 2.8. Effects of strip thickness and number of strips on the shear stress of small-scale wood composite poles.
28
little difference in the bending stress for different strip thickness and number levels.
Although the two thinner shell poles were failure at shear, the shear stress values were
listed in Table 2.5 due to the small difference between the shear stress values of the
thinner poles and normal stress values of the thicker poles.
Table 2.6 lists the flexural properties of spruce and southern yellow pine solid
poles that were bonded by two pieces of lumber and processed to polygonal shapes. The
strength of the composite poles was comparable to that of bonded solid poles. In the 2.0
cm groups, the strength of 6-, 9-, and 12-sided poles accounted for 99, 82, and 90 percent
of corresponding solid ones, respectively.
Table 2.5. Maximum bending stress of small-scale wood laminated composite poles.
Bending Stress (MPa) Strip
Thickness (cm) 6-strip 9-strip 12-strip
1.0* 96.27 (1.16)** 91.85 (1.68) 52.91 (6.27)
1.5* 96.76 (5.69) 90.02 (0.89) 80.53 (5.23)
2.0 101.37 (7.64) 80.84 (1.27) 99.46 (5.98)
2.5 106.16 (1.34) 108.86 (5.56) 97.80(12.53)
* The poles in these two thickness levels failed in shear at the clamped end.
** Values in parentheses are standard deviation.
Table 2.6. Flexural properties of the small-scale solid poles.
MOR (MPa) MOE (109Pa) Species
6-sided 9-sided 12-sided 6-sided 9-sided 12-sided
Spruce 61.59(13.65)* 68.06 (4.38) 72.87 (1.15) 5.35 (0.744) 6.42 (0.758) 6.24 (0.786)
SYP** 112.4 (2.15) 99.19 (4.37) 110.7(5.51) 8.12 (0.593) 7.95 (0.062) 7.65 (0.455)
* Values in parentheses are standard deviation.
** Southern yellow pine
29
2.5.2 Modulus of Elasticity
The Youngs modulus values of small-scale composite poles of different strip
thickness and NOS levels are presented in Table 2.7. Table 2.6 lists the modulus of
spruce and southern yellow pine solid poles. Variations existed among different NOS
and strip thickness levels in the MOE of composite poles, as shown in Figure 2.9. In
general, the Youngs modulus of composite poles was lower than those of solid poles
with the same species. The reduction ranged from 0 up to 60 percent. Errors existed
when prepared the strips that composed the poles. The integrity of the poles might thus
be affected and a reduction in stiffness could be expected. Statistical results show that
strip thickness was not correlated to the MOE values of the composite poles (p = 0.3928).
The average MOE values were 6.2, 6.6, 5.7, and 5.9 TPa for strip thickness of 1.0, 1.5,
2.0, and 2.5 cm, respectively. There were no significant differences among the MOE
values in the LSD test.
Table 2.7. Modulus of elasticity of small-scale wood laminated composite poles.
MOE (109Pa) Strip
Thickness (cm) 6-strip 9-strip 12-strip
1.0 5.77(0.59) 4.73(0.31) 6.49(1.02)
1.5 5.32(2.33) 6.49(0.82) 6.45(1.40)
2.0 5.71(0.58) 5.58(0.73) 6.38(0.17)
2.5 6.21(0.89) 6.10(0.67) 6.66(0.33)
* Values in parentheses are standard deviation.
Tests show that NOS had a significant effect on Youngs modulus of the
composite poles (p = 0.0002). The average MOE values were 5.3, 5.6, and 7.4 MPa for
NOS of 6, 9, and 12. The 12-sided MOE was significantly higher than that of 6- or 9-
30
sided. The higher MOE of the 12-sided MOE may result from the effects of the glue-
lines. There are 12 glue-lines one each of the 12-sided poles. The stiffness of the glue-
line is higher that that of solid wood and allowed the composite pole to have higher MOE
values.
Table 2.8 lists the Youngs modulus values of full-size composite poles. When
comparing these MOE values with those in Tables 2.6 and 2.7, it is noted that the
stiffness of full-size composite poles was much higher than that of small-scale composite
poles or solid poles. Full-size and small-scale composite poles basically belong to the
same materials and would have the same stiffness. The addition of disks and fillings in
the hollow part of the clamp side may change the properties of the full-size composite
poles. In other words, the fillings below the ground-line may enhance the bending
stiffness of the poles. Statistic analysis results show that strip thickness (p = 0.3087) and
number (p = 0.7529) were not correlated to the MOE. The average MOE values were
10.8, 12.1, and 12.5 TPa for strip thickness of 1.91, 2.86, and 3.81 cm; and the average
for 9 and 12 NOS were 11.6 and 11.9 TPa. There were no significant differences among
different strip thickness levels and among different NOS levels.
Table 2.8. Modulus of elasticity of full-sized laminated composite poles.
Modulus of elasticity (109Pa) Strip thickness
(cm) 9-strip poles 12-strip poles
1.91 10.61(0.277)* 10.90 (2.578)
2.86 12.28(3.426) 12.84 (2.494)
3.81 12.04 (0.502) 12.92 (1.232)
* Values in parentheses are standard deviation.
31
0.0
3.0
6.0
9.0
12.0
Strip Thickness (cm)
MO
E (T
Pa)
12 Strips
9 Strips
6 Strips
2.5 2.0 1.5 1.0
Figure 2.9 Effects of strip thickness and number on the modulus of elasticity of small-scale wood laminated composite poles.
32
2.5.3 Glue-Line Shear
The shear strength and wood failure in both dry and wet conditions in the glue-
line shear test of small-scale composite poles are listed in Tables 2.9 and 2.10. In
general, shear strength in the dry condition decreased with an increase of strip thickness.
One of the exceptions is the 12-strip poles with 1.5 cm thick strip, the shear strength of
which was much higher than the other groups. The percentage of wood failure of this
group is lower than others in the same thickness level (Table 2.10). Statistic analysis
shows that strip thickness effects were significant on shear strength and wood failure in
both wet and dry conditions. In the dry condition, average shear strength values were
9.54, 8.80, 7.98, and 7.56 MPa for thickness levels of 1.0, 1.5, 2.0, and 2.5 cm,
respectively; and the corresponding wood failure values were 50, 63, 69, and 72 percent
for the four thickness levels, respectively. Figure 2.10 shows the effects of variables on
samples shear strength and Figure 2.11 gives the effects of variables on wood failure in
the dry condition.
Table 2.9. Glue-line shear strength values before and after water soaking of small-scale composite poles.
Shear in dry condition (MPa) Shear in wet condition (Mpa) Strip
thickness 6-strip 9-strip 12-strip 6-strip 9-strip 12-strip
2.5 7.33 (0.33)* 8.15 (1.15) 6.30 (1.08) 5.13(0.14) 5.36(0.33) 4.85(1.05)
2.0 5.96 (0.54) 7.68 (0.49) 10.29 (2.08) 4.61(0.26) 5.20(0.20) 4.81(0.26)
1.5 7.84 (0.88) 9.71 (0.03) 8.85 (1.45) 5.58(0.22) 5.34(0.69) 4.96(0.99)
1.0 10.08 (0.79) 10.15 (0.63) 8.39 (1.05) 7.01(1.84) 4.97(0.31) 5.33(0.20)
* Values in parentheses are standard deviation.
The greater shear strength of poles with thinner strips may be due to the fact that
thinner shells received more pressure than the ones with thicker shells. During the
making of the poles, the same force was added to the same molds. The thinner strips may
33
have greater pressure in the glue-line and have better bonding conditions because of their
lower contact area between them. This indicates that sufficient pressure is necessary
when making composite poles. Excessive pressure may cause the problem of squeezing
glue out of the glue-line and lowering the bonding strength but that was not the case in
this study. Among the four thickness levels, LSD results showed that the shear strength
of each level was significantly different from the others, meaning that shear strength
increased with the decrease of strip thickness i.e., increase of pressure.
Table 2.10 Percentage of wood failure in the glue-line shear test of wood composite poles.
Shear in dry condition (%) Shear in wet condition (%) Strip
thickness 6-strip 9-strip 12-strip 6-strip 9-strip 12-strip
2.5 73.81 (7.30)* 68.75(12.37) 72.00 (7.17) 67.17 (6.76) 70.83(15.28) 46.67(13.33)
2.0 72.81(14.35) 75.92 (7.30) 57.72(12.80) 72.28(18.51) 54.89 (8.60) 44.92(13.81)
1.5 63.61(10.21) 70.22 (5.01) 54.50 (8.01) 47.50(12.50) 24.03(13.18) 46.25 (8.33)
1.0 52.92(35.22) 54.06 (9.67) 54.42 (3.88) 48.42(24.12) 38.75 (5.73) 35.14 (4.57)
* Values in parentheses are standard deviation.
Figures 2.10 and 2.11 show that shear strength increased and wood failure
decreased as strip thickness decreased. It can be seen that high shear strength between
thin strips corresponded with low wood failure and low shear strength between thick
strips with high wood failure.
After the 2-hour boiling test, the shear strength was reduced to 5.11, 4.84, 5.30, and
5.77 MPa, and the wood failure was reduced to 41, 39, 55, and 62 percent for the four
thickness levels, respectively. The poles with strip thickness from 1 to 2.5 cm lost 46, 45,
34, and 24 percent of the original strength, respectively. Thinner poles lost more strength
after the treatment. In the wet condition, the poles with 2.5 cm strip thickness had the
34
11.5
2
2.5 6
9
12
0
2
4
6
8
10
12
Shea
r Stre
ngth
(MPa
)
Strip Thickness (cm) Strip N
umber
Figure 2.10. Effects of strip thickness and NUMBER OF STRIPS on the glue-line shear strength of wood composite poles.
11.5
22.5
6
9
12
0
10
20
30
40
50
60
70
80
Woo
d B
reak
age
(%)
Strip Thickness (cm)
Strip Number
Figure 2.11. Effects of strip thickness and NUMBER OF STRIPS on
wood failure in the glue-line shear test of wood composite poles.
35
highest shear value and was significant different from the others. There were no
differences for the shear strength between the poles with thickness values of 2.0 and 1.0
cm, but both were higher than the ones at 1.5 cm thickness. Poles with thick strips still
had higher wood failure, indicating they are more durable than poles with thin strips.
Figures 2.12 and 2.13 show these trends.
Another factor that affects the shear strength and wood failure is the grain
direction of the strips that form the glue-line. For the species used in this study, southern
pine, earlywood and latewood alternatively appear on the cross section. The best scheme
for the glue bond consideration is that the grain planes on both surfaces are parallel to the
glue-line plane. Under this condition, the materials on the two bonding surfaces are
uniform and good bonding quality may be obtained. In this case, the tangential direction
of a wood strip coincides with the radial direction of the pole and the radial direction of a
wood piece becomes tangential in the pole. Another advantage of this arrangement is
that the tangential shrinkage of the pole will be minimized due to less shrinkage and
swelling in the radial direction of the wood. The worst case for the glue bond is when the
annual rings on both sides of the glue-line are perpendicular to the glue-line. The
hardness of latewood is greater than that of the earlywood. If two latewood rings match
up in the glue-line, they will affect the bonding of the earlywood rings next to the
latewood rings. Also the tangential direction of the wood strips coincides with that of the
pole, more shrinkage and swelling in the pole is expected. The effects of wood growth
ring direction and the gluability of earlywood and latewood had great effects on the
physical and mechanical properties of composite poles and will be further studied in the
future.
36
11.5
22.5
6
9
120
1
2
3
4
5
6
7
8
She
ar S
treng
th (M
Pa)
Strip Thickness (cm)Str
ip Num
ber
Figure 2.12. Effects of NUMBER OF STRIPS and thickness on the shear strength of wood composite pole samples after a 2-hour boiling test.
11.5
22.5
6
9
12
0
10
20
30
40
50
60
70
80
Woo
d Br
eaka
ge (%
)
Strip Thickness (cm)
Strip Number
Figure 2.13. Effects of strip thickness and number on the wood failure of composite
poles in the shear test after a 2-hour boiling treatment.
37
2.6 Conclusions Full- and small-scale wood composite poles were fabricated, tested and analyzed.
Small-scale poles were tested to failure and the glue-line shear strength in both wet and
dry conditions were obtained from the unchanged properties of previously tested poles.
The full-size poles were not tested to failure due to the need for subsequent experiment
on these poles. Strain gages were attached to the full-size poles to obtain the strain
during the test. Spruce and southern yellow pine solid poles were also processed and
tested as controls for the analysis of composite poles. Strip thickness and NOS were the
factors that affected the mechanical properties of composite poles:
1. Strip thickness had negative effects on the glue-line shear stress in both dry and
wet conditions. Strip thickness was not correlated with the shear stress at the
clamped end of the small-scale composite poles, the maximum bending stress of
the small-scale composite poles, and Youngs modulus of both full- and small-
scale composite poles.
2. NOS is another important factor in determining the mechanical properties of
composite poles. With an increase of NOS, the modulus of elasticity increased. It
had no effects on the glue-line shear strength properties. More strips in a pole
incurred more processing errors and resulted in poor bonding quality and pole
integrity.
3. The Two-hour heating + Two-hour boiling treatment resulted in a reduction in
shear strength and an increase in glue-line failure. Thinner strips lost more shear
strength after the treatment and had low durability.
38
4. The modulus of elasticity of small-scale wood composite poles was inferior to
that of solid poles with the same species. The modulus of elasticity of full-size
wood composite poles was superior to that of solid poles.
2.7 References Adams, R.D., S. Mateer, G.P. Krueger, A.E. Lund, D.D. Nicholas. 1981. Composite wood utility poles. EL-1745 Research Project 796-1. Prepared for Electric Power Research Institite. 3412 Hillview Avenue, Palo Alto, California 94304. American Society for Testing and Materials. 1996. Standard methods of static test of wood poles, D 1036-58(64). Erickson, R.W. 1995. Hollow veneered pole. U.S. Patent. Number 5,438,812.
39
CHAPTER 3
THEORETICAL MODELS OF LAMINATED WOOD COMPOSITE POLES
3.1 Introduction
In the analysis of bending beams, the classical Bernoulli-Euler theory has long
been used as a convenient approximation for slender beams in structural analysis and
design (Rehfield and Murthy 1982). The main assumption in this theory is that the
transverse plane that is normal to the beam middle plane remains normal during bending.
This assumption implies that the transverse shear strain and deformation are neglected.
The Bernoulli-Euler theory may lead to serious discrepancies in cases of deep beams with
small slender ratios (L/h) (Kant and Gupta 1988). The refinement of this theory has been
attracting attention for almost one and a half of century (Kathnelson 1996). Among these
efforts, Timoshenko (1921) improved the validity of the theory by incorporating the
effect of transverse shear into the governing equations. This theory assumed that cross
section remains a plane after bending and the shear stress is uniform through the
thickness of the beam. In order to recognize the nonuniform shear stress distribution at a
section, a factor is introduced into the shear stress formula. After this improvement, the
classical theory can be used to calculate the deflection for short as well as long beams.
One of the earliest studies of shear effects on wood was done by Biblis (1965).
Two methods were used in his study, i.e., an elementary direct method and the energy
method. In the direct method, it was assumed that all cross sections were free to deform
and the curve due to shear was represented by two straight lines, whereas the energy
method has no such assumptions and is thus more accurate. His study shows that the
40
percentage of deflection due to shear is dependent on the span-to-depth ratios and could
be as high as more than 50 percent when the ratio is 8:1.
Wood laminated composite poles are thick-wall beams with a polygonal cross
section. The hollow beams have sufficient strength and stiffness properties but relatively
low weight, as compared to solid wood poles. The merits that wood composite poles
have, such as produced from renewable natural resources, broad material and material
size requirements, and easy treatment make this hollow beam superior to poles and beams
from other materials as well as solid wood poles. In addition to the applicability for utility
poles, hollow wood composite beams may find applications in pillar, post, and
engineering beams. To enhance the material and structural efficiencies, theoretical
research is needed. The present study is to construct theoretical models through two
methods (high-order differential equation, Timoshenko beam theory) to assess the stress
and strain properties of this new engineered wood product. The high-order differential
equation method was based on the energy method, i.e. the principle of minimum potential
energy of wood composite poles. This general approach has been used in other literatures
in solving beams and plates in bending. It is formulated in terms of scalar quantities such
as work and energy. An advantage of energy methods is that they avoid some extraneous
detail, such as geometric manipulation of deflection components. Another advantage is
their ability to yield approximate solutions for problems too complicated to be solved
exactly. The objective of this part of the study was to develop a theoretical model using
high-order differential equations and the principle of minimum potential energy to assess
and predict the properties of wood composite poles.
41
3.2 High-Order Differential Equations
The target composite pole of this study is composed of a number of wood strips
bonded with an adhesive. The thickness of the strips are less than the radius of the circle
outside the cross section, thus the poles are hollow inside. Figure 3.1 shows a typical
design of a polygonal wood composite pole and its right-hand set of coordinate axes x, y,
and z. The corresponding axial displacements are u, v, and w. The NOS in one pole is 3n,
where n is 1, 2, 3, etc. The pole shown in the Figure 3.1 is one of the target poles
analyzed in this study. It has 12 strips and 12 glue lines.
Figure 3.1. A schematic diagram of a wood composite pole and its coordinates.
r R
z, w
x,
y, v
The lateral displacement (w) of the pole was assumed to consist of four parts: the
elementary theories of normal and shear displacements of the wood strips and glue layers.
In this section, the normal and shear strain energies for wood and glue layers were
42
derived. Since the thickness of each glue layer is much thinner than that of a wood strip,
the glue layer thickness was neglected in the analysis of strain energy of wood strips. The
strain energy stored in glue layers was analyzed separately from wood strips.
Figure 3.2. A loading system and shear and moment distribution of a cantilever beam.
PL + 0.5p0L2 (c)
A
A
z
x
B
(a)
B
P + p0L
p0 P
L
(b)
A B
P P + p0L
According to the theories, the normal and shear stresses of the pole can be
expressed as
(3.1) Ix= Mz
(3.2) zdAxy == IbVQ
bIdxdM R
z
1
43
where M is the bending moment, I is the moment of inertia of the cross section of the
pole, V is the vertical shear force, b is the width of the pole, and Q is the first moment.
The strain energy density function for a beam, in Cartesian coordinate system, is defined
as
(3.3) xx 2W 1=
(3.4) xyxyW 2=1
where
2
2
dxwdz
dxdu x
x == (3.5)
Gxy
xy
= (3.6)
Thus, the strain energy functions becomes
(3.7) 2 ) zEEW xxx === 222
2
(21
21
21
dxwd
(3.8)
22
222
21
21
21
bGIQV
GW xyxyxy ===
Since (elementary mechanics), Equation 8 becomes 33
dxwdEIV =
(3.9) .)3(2222 dxGbGIW == 2
32212
221 wdQE
b
QV
44
After integrating Equations 7 and 9 with respect to y and z and substituting the value of I,
we have the normal strain energy and shear strain energy stored in the pole as the
followings:
UEI d w
dxdx
L
= 22
20
2( ) (3.10)
UEG
d wdx
dxQb
dydzL
A = 2 3 30 2
2
22( ) (3.11)
Thus we obtained the general expressions of the strain energies for both the wood and
glue layers. Let kQb
dydzA
1
2
2= , then shear strain energy for the whole pole has the form
Uk E
Gd wdx
dxL
= 1 2 3 30 22 ( ) (3.12) In the design of this study, the pole has 3n strips, and thus 3n glue layers. Take the
12-strip pole as an example, the pole has 12 strips and glue layers, as shown in Figure
3.3. The strain energy of each glue layer is the sum of strain energy caused by normal and
shear strain. And the total strain energy of the glue layers is the sum of the strain energy
for each glue layer:
. LLBBAA
LLLLBBBBAAAAg
UUU
UUUUUUU
+++=++++++=
LL
Since some of them are equal, the total strain energy of the glue layers can be expressed
as
dxdx
wdkdxdx
wdk
UUUUU
LL
DDCCBBAAg
20 3
3
72
0 2
2
6 )()(
2442
+=+++=
(3.13)
45
where
k E I I I
k k k k k k
kEG
kQ
t IdA
kQ
t IdA
kQ
t IdA
kQ
t IdA
g g g g
g
g
g
gA
g
gA
g
gA
g
gA
6 1 2
7 5 1 2 3 4
5
2
41
2
21
32
2
22
23
2
23
14
2
24
2 2
2
2
4
4
2
= + += + + +
=
=
=
=
=
( )
( )3
and Ig1, I g2, and I g3 are the moment of inertia of glue layers, Qg1, Qg2, Qg3, and Qg4 are
the first moment of each of the glue lines, Eg is the Youngs modulus of glue, Gg is the
rigidity of glue, and A is the area of the cross section.
G
CD
E
B C
A
F
D A'
B
J JLK
IHG
I
L
K
FE
H
z
y
Figure 3.3. A schematic diagram of the cross section of a 12-strip pole shell.
46
Two external forces are applied to the pole system. They are body force of pole
(p0) and the applied concentrated load (P) at the free end. Then the work done by the
external force is as followings
(3.14) H p wdx PwL= 00 ( )L where
H - work done by the external force
p0 - body force of the pole
w - transverse displacement along the length of the pole L
The total potential energy is given as
= + + +U U U Hg (3.15)
Substitute Equations 10, 12, 13, and 14 into Equation 15 and rearrange, the total potential
energy is given by
= + k d wdx dx kd wdx
dx p wdx Pw LL L L82
202
9
3
302
00( ) ( ) ( ) (3.16)
where
k EI
kk E
Gk
8 6
91
2
7
12
2
= +
= +
k
The principle of minimum potential energy states that of all the displacements which
satisfy the boundary conditions of a structural system, those corresponding to stable
equilibrium configurations make the total potential energy a relative minimum.
According to this principle, the system is in equilibrium when the first variation in
vanishes. Thus the equilibrium condition is
47
= =x dx 0
or
kd wdx
d wdx
dx kd wdx
d wdx
dx p wdx P w LL L L82
20
2
2 9
3
30
3
3 002 2 + ( ) ( ) ( ) 0= (3.17)
Equation 17 yields one differential equation, which is the governing differential equation
for the pole loading system.
kd wdx
kd wdx
p9
6
6 8
4
40
20+ = (3.18)
with boundary conditions
[ )]kd wdx
kd wdx
Px L9
5
5 8
3
3 2 = = (3.19)
( )kd wdx
kd wdx x L8
2
2 9
4
4 0 =| = (3.20)
0| 033
8 ==xdxwdk (3.21)
The other boundary conditions may be as followings
(3.22) w x| = =0 0
(3.23) w x'| = =0 0
kd wdx x L8
2
2 0| = = (3.24)
Then the following solution is obtained w c c x c x c x
kp x c e c ek x k x= + + + + + + 1 2 3 2 4 3
80
45 6
148
10 10 (3.25)
48
where
kkk10
8
9=
and c to are constants and given as follows: 1 c6
Ck p L P e e p
k k e e
k L k L
k L k L110 0 0
8 104
10 10
10 10
22
= + ++
( )( )
( )
Cp L P
k k20
8 1022
= +
Cp L PL
kp
k k30
2
8
0
8 102
28 2
= + +
Cp L P
k40
812= +
Ck p L P e p
k k e e
k L
k L k L510 0 0
8 104
15
10 102= + +
( )
( )
Ck p L P e p
k k e e
k L
k L k L610 0 0
8 104
15
10 102= + ++
( )
( )
3.3 Solutions Based on Timoshenko Beam Theory
U, V, and W are the displacement at x, y, z directions, respectively. Since U is a
function of (x, y, z), we expand U into a Tylor series (Washizu 1968, Kant and Gupta
1988) about z = 0:
... )(!21 )()0 , ,() , ,( 202
2
0 ++
+= == zzUz
zUyxUzyxU zz (3.26)
After retaining the first two terms of Equation 26,
10 UzUUrrr += (3.27)
49
where U . Equation 27 is an expression that includes the effect of transverse
shear deformation. Two assumptions were made: (1) a cross section perpendicular to
undeformed central line remains perpendicular to the deformed locus; (2) the
displacement is small. Then we have
31111 iwiurrr +=
wWVuzuU ,0 , 1 ==+= 1xz1 u w' ,'u z u' +=+= x (3.28) The total strain energy of the beam may be expressed as
(3.29) PwwdxpdxdL += 0
0C
xzxzxx ydz)(
According to principle of minimum potential energy, the system is in equilibrium when
the first variation in vanishes:
(3.30) 0)(0
0V
x =+= wPwdxpdxdydzL
xzxzx
Substitute Equation 28 into Equation 30, we obtain the following equation
0 -dx ] w - ) u w' ( u ' u [ 01L
01 =+++ wP pQM N (3.31)
where
, , dydzNS
x= zdydzMS
x=
dydzQS
xz= (3.32a, b, c) N is the axial force, M the bending moment, and Q the shear force. Integrate Equation 31
and rearrange, the following Equation may be obtained
50
+++ dxwpQuMQuNL
])'()'('[ 00
1
0][])([ 011 =++++ == xLx uMwQuNuMwQPuN (3.33) Then the governing differential equations are as followings:
(3.34a) 0' pQ = (3.34b) QM =' (3.34c) 0'=Nand boundary conditions P = Q |x = L, also
u(0) = w(0) = u1(0)|x=0 = 0
M| x=L = 0
Based on these boundary conditions, Equation 34 may be solved. Substitute Equation 28
into Equation 32, we have
=+==S S
x EAudydzzuuEdydzN ')''( 1
===S S
xx EIudydzzEzdydzM '12
+===S S
xzxz uwGkdydzGEdydzQ )'( 1 (3.35a, b, c) where k is a Timoshenko constant and determined by the following formula (Shames and
Dym 1985):
22
)1220()1)(67()1)(1(6
mmmk
++++
++= (3.36)
51
where m = D/d. D is the diameter of circumscribe circle of the cylinder, and d is the
diameter of the inscribe cycle, v is the Piosson ratio. Substitute Equation 35 into
Equation 34 and notice that no axial loads were added,
EIu1 = kGA (w + u1) (3.37)
KGA[w + u1] = - p0 (3.38)
Take derivative of Equation 37 and substitute Equation 38, we have
EIu1 = kGA(w + u1) = p0
Integrate the above equation three times, we have
322
13
0 21
61 CxCxCxpEIu +++= (3.39)
where C1, C2, C3 are constants. Solve Equation 39 using boundary conditions, we obtain
the deflection function of a cantilever beam subjected to body and concentrated loads:
xkGALpPx
kGAp
EILpPLx
EILpPx
EILpw 020
20304
30 )
242(
624+++++= (3.40)
and the maximum deflection is
kGALp
kGAPL
EILp
EIPLw
283
20
40
3
max +++= (3.41)
It is noted that the first and second terms on the right side of Equation 41 are the bending
parts of the total deflection caused by concentrated and body force loads, while the last
two terms are the shear parts of the total deflection. It is also noted that the EI and GA in
Equations 40 and 41 are the sum of both wood strips and glue layers so that the glue layer
effects may be taken into account in the total deflection.
52
3.4 Experimental Study
To validate the applicability of the theoretical models and to predict the
deflection, an experimental investigation was conducted on the reduced- and full-size
composite poles. The experiment validation data was from Chapter 2. The species was
southern yellow pine. Strip thickness and NOS are the two variables of the two kinds of
composite poles. For the small-scale composite poles, strip thickness levels were 1.0 cm
(0.4 in), 1.5 cm (0.6 in), 2.0 cm (0.8 in), and 2.5 cm (1.0 in), each of which had 6, 9, and
12 NOS. The length of the poles was 1.06 m (48 in). For the full-size poles, the strip
thickness levels 1.9 cm (0.75 in), 2.9 cm (1.125 in), and 3.8 cm (1.5 in) and NOS was 9
and 12. Pole length was 5.16 m (20 ft.). There were three replications of each
combination of strip thickness and number levels.